A single molecule magnet to single molecule magnet transformation via a solvothermal process: Fe4Dy2 →Fe6Dy3.
Chen, Sihuai; Mereacre, Valeriu; Anson, Christopher E.; Powell, Annie K.; Dalton transactions (Cambridge, England : 2003) 45 (2015) 98–106; doi:10.1039/c5dt03909f

data_7037399
_publ_section_title
;
 A single molecule magnet to single molecule magnet transformation via a
 solvothermal process: Fe4Dy2 \\rightarrow Fe6Dy3.
;
_journal_issue                   1
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              98
_journal_page_last               106
_journal_paper_doi               10.1039/c5dt03909f
_journal_volume                  45
_journal_year                    2015
_chemical_formula_moiety         'C76 H78 Fe4 N12 O42 Y2, 3(C2 H3 N)'
_chemical_formula_sum            'C82 H87 Fe4 N15 O42 Y2'
_chemical_formula_weight         2355.88
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2015-10-06 deposited with the CCDC.
2015-11-01 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 95.539(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   31.177(4)
_cell_length_b                   15.660(2)
_cell_length_c                   20.673(3)
_cell_measurement_reflns_used    9852
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      31.35
_cell_measurement_theta_min      2.66
_cell_volume                     10046(2)
_computing_cell_refinement       'Apex2 (Bruker AXS Inc., 2005)'
_computing_data_collection       'Apex2 (Bruker AXS Inc., 2005)'
_computing_data_reduction        'Apex2 (Bruker AXS Inc., 2005)'
_computing_molecular_graphics    'Diamond 2.1 (Crystal Impact, 1998)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'Apex2 (Bruker AXS Inc., 2005)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector_area_resol_mean 8.333
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measurement_device_type  'Bruker SMART Apex'
_diffrn_measurement_method       'CCD area detector, \w-scans'
_diffrn_radiation_monochromator  silicon
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.80000
_diffrn_reflns_av_R_equivalents  0.0330
_diffrn_reflns_av_unetI/netI     0.0247
_diffrn_reflns_laue_measured_fraction_full 0.996
_diffrn_reflns_laue_measured_fraction_max 0.985
_diffrn_reflns_limit_h_max       40
_diffrn_reflns_limit_h_min       -40
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            57445
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.985
_diffrn_reflns_theta_full        29.000
_diffrn_reflns_theta_max         31.400
_diffrn_reflns_theta_min         2.228
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    1.129
_exptl_absorpt_correction_T_max  0.965
_exptl_absorpt_correction_T_min  0.729
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS 2.10 (Bruker AXS Inc., 2005)'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.558
_exptl_crystal_description       block
_exptl_crystal_F_000             4808
_exptl_crystal_preparation       'Magnetic properties'
_exptl_crystal_recrystallization_method 'Re-crystallisation from solvent: '
_exptl_crystal_size_max          0.230
_exptl_crystal_size_mid          0.080
_exptl_crystal_size_min          0.050
_refine_diff_density_max         1.466
_refine_diff_density_min         -0.931
_refine_diff_density_rms         0.136
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.028
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     553
_refine_ls_number_reflns         11454
_refine_ls_number_restraints     23
_refine_ls_restrained_S_all      1.029
_refine_ls_R_factor_all          0.0884
_refine_ls_R_factor_gt           0.0778
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1280P)^2^+85.9163P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2179
_refine_ls_wR_factor_ref         0.2302
_reflns_Friedel_coverage         0.000
_reflns_number_gt                9798
_reflns_number_total             11454
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5dt03909f2.cif
_cod_data_source_block           mc1287
_cod_depositor_comments
'Adding full bibliography for 7037399--7037400.cif.'
_cod_database_code               7037399
_shelx_estimated_absorpt_t_min   0.781
_shelx_estimated_absorpt_t_max   0.946
_shelxl_version_number           2014-3
_shelx_res_checksum              92402